new twist on artificial muscles - pnas 12-خ¼m-diameter yarn provided 250آ°/mm of rotation at...
Post on 23-May-2020
Embed Size (px)
SPECIAL FEATURE: PERSPECTIVE
New twist on artificial muscles Carter S. Hainesa,1,2, Na Lia,1, Geoffrey M. Spinksb, Ali E. Alieva, Jiangtao Dia, and Ray H. Baughmana,2
Edited by Joseph M. DeSimone, University of North Carolina at Chapel Hill and Carbon, Chapel Hill, NC, and approved August 19, 2016 (received for review May 22, 2016)
Lightweight artificial muscle fibers that can match the large tensile stroke of natural muscles have been elusive. In particular, low stroke, limited cycle life, and inefficient energy conversion have combined with high cost and hysteretic performance to restrict practical use. In recent years, a new class of artificial muscles, based on highly twisted fibers, has emerged that can deliver more than 2,000 J/kg of specific work during muscle contraction, compared with just 40 J/kg for natural muscle. Thermally actuated muscles made from ordinary polymer fibers can deliver long-life, hysteresis-free tensile strokes of more than 30% and torsional actuation capable of spinning a paddle at speeds of more than 100,000 rpm. In this perspective, we explore the mechanisms and potential applications of present twisted fiber muscles and the future opportunities and challenges for developing twisted muscles having improved cycle rates, efficiencies, and functionality. We also demonstrate artificial muscle sewing threads and textiles and coiled structures that exhibit nearly unlimited actuation strokes. In addition to robotics and prosthetics, future applications include smart textiles that change breathability in response to temperature and moisture and window shutters that automatically open and close to conserve energy.
artificial muscles | actuators | carbon nanotubes | yarns | textiles
The Need for Better Artificial Muscles Electromagnetic motors and actuators have enabled an impressive array of robotic and prosthetic devices. Unfortunately, these actuators are heavy and cannot provide the large contractile strokes in the small foot- print that natural muscles do. These compromises have led to robotics that can greatly overpower natural or- ganisms in terms of raw force generation but that have difficulty achieving the fine motion and soft actuation required for complex tasks, like recreating human-like facial gestures or catching a ball. Additionally, nature tends to achieve high dexterity across large working envelopes by using kinematic chains of actuators. The human arm is a good example, beginning at the shoulder, and ultimately supporting more than 7 de- grees of freedom in the arm and up to 27 additional degrees of freedom in the hand (1, 2). This arrangement is a compounding issue for robotics using heavy actu- ators and motors, which must rely on increasingly larger
actuators toward their base to support actuator mass at the extremities.
Numerous types of “artificial muscles” have been developed to try to bridge this gap. Because our goal is to consider lightweight artificial muscles that offer similar shape and functionality as natural muscle, we here restrict discussion to artificial muscle fibers. Al- though some types of artificial muscle fibers can gen- erate 53 times higher maximum contractile work per cycle, 85 times higher typical contractile power density, and much larger strokes than can natural muscle (3–6), no artificial muscle fiber can yet provide the high energy conversion efficiencies, self-reparability, and billions of reversible actuation cycles of natural muscles (3, 7).
Wires made from shape memory alloys have seen use as artificial muscles since their popularization in the 1970s. When heated thermally or electrothermally by Joule heating, these muscles can provide large spe- cific work per cycle, exceeding that of natural muscle by more than 20 times (∼930 vs. 40 J/kg). However, these
aThe Alan G. MacDiarmid NanoTech Institute, Department of Chemistry, University of Texas at Dallas, Richardson, TX 75080; and bSchool of Mechanical, Materials andMechatronic Engineering, Australian Research Council (ARC) Centre of Excellence for Electromaterials Science, University of Wollongong, Wollongong, NSW 2522, Australia Author contributions: C.S.H., N.L., A.E.A., J.D., and R.H.B. designed research; C.S.H., N.L., A.E.A., and J.D. performed research; C.S.H., N.L., G.M.S., A.E.A., J.D., and R.H.B. analyzed data; and C.S.H., N.L., G.M.S., A.E.A., J.D., and R.H.B. wrote the paper. Conflict of interest statement: Provisional patent 62/371,744, “Twisted, plied, uniformly coiled, and non-uniformly coiled artificial muscles for textile applications,” was filed on August 6, 2016. This article is a PNAS Direct Submission. 1C.S.H. and N.L. contributed equally to this work. 2To whom correspondence may be addressed. Email: email@example.com or firstname.lastname@example.org. This article contains supporting information online at www.pnas.org/lookup/suppl/doi:10.1073/pnas.1605273113/-/DCSupplemental.
www.pnas.org/cgi/doi/10.1073/pnas.1605273113 PNAS | October 18, 2016 | vol. 113 | no. 42 | 11709–11716
S P E C IA
L F E A T U R E :
P E R S P E C T IV
http://crossmark.crossref.org/dialog/?doi=10.1073/pnas.1605273113&domain=pdf mailto:email@example.com mailto:firstname.lastname@example.org http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1605273113/-/DCSupplemental www.pnas.org/cgi/doi/10.1073/pnas.1605273113
wires normally provide less than 8% contraction, with 4–5% being typical, and their response is relatively binary and hysteretic (8, 9), making it hard to controllably achieve intermediate contraction states. Coiling these shape memory alloy wires increases stroke to as much as twice their initial coil length (10), but these springs are difficult to fabricate into tight coils, leading tomuscles with low force generation. Shape memory polymers may also be used as artificial muscle fibers, but they typically provide low work capacity, and, like shape memory alloys, their contraction is difficult to control precisely (11, 12).
A host of other remarkable actuating materials and actuation processes have been extensively investigated. These actuators in- clude, for example, piezoelectric ceramics and polymers (13–15), electrostatic actuators based on deformable capacitors (16, 17), electrochemically doped conducting polymers (18), and cantilever- based ionic-polymer metal composites (19, 20). However, because it is challenging to use these alternative actuator materials and pro- cesses in small-diameter artificial muscle fibers, we will restrict pre- sent discussion to recently discovered high-performance artificial muscle fibers whose remarkable properties depend on inserted twist.
The Path to Twisted Artificial Muscles In recent years, a new class of muscles has emerged based on highly twisted fibers. These muscles can provide powerful strokes at more than 30% reversible contraction (4), torsional actuation that can spin rotors at more than 100,000 rpm (21), and specific work during contraction of 2.48 kJ/kg, which is more than 50 times that of natural skeletal muscle. In the following sections, we ex- plore the mechanisms that underlie these muscles and the op- portunities they bring forth.
The first demonstration of a highly twisted artificial muscle was the 2011 discovery of torsional actuation from carbon nanotube (CNT) yarns (22). When twisted and immersed in an electrolyte, a 12-μm-diameter yarn provided 250°/mm of rotation at speeds up to 590 rpm when charged electrochemically. In 2012, CNT yarns were further shown to provide tensile actuation after twisting to such an extreme degree that the fiber spontaneously formed coils (5). These coils mechanically behave like tight springs and can provide tensile contraction of ∼7.3% when pristine coiled CNT yarns are heated to incandescent temperatures in an inert envi- ronment. More practically, by infiltrating CNT yarns with a guest material having a large coefficient of thermal expansion, these hybrid CNT yarns could provide torsional and tensile actuation in lower temperature ranges. For instance, a coiled CNT yarn infil- trated with paraffin wax delivered over 5% contractile stroke when heated to 200 °C (5). More recently a coiled, silicone rubber- infiltrated CNT yarn has provided a tensile stroke of more than 34% when heated electrothermally and 50% when actuated by solvent absorption.
Twisted and coiled CNT yarns have provided unprecedented torsional and tensile work capacities, but the high cost of fabri- cating these CNT fibers has limited their application. In this area, a key breakthrough came in 2014 with the development of poly- mer-based twisted fiber muscles. These artificial muscle fibers could be easily fabricated by simply twisting widely available, low- cost materials like fishing line and sewing thread. When twisted to form coils, these muscles provided more than 30% tensile stroke when heated, operated without hysteresis, and provided millions of cycles of stroke without significant degradation (4).
Twisted Muscle Mechanisms The process of making a twisted artificial muscle begins with a precursor fiber that has at least some degree of internal alignment.
In the case of carbon nanotube yarns, this alignment comes from the bundles of nanotubes that are oriented along the fiber di- rection during fabrication to provide strength to the yarn. Polymer muscles similarly use high strength fibers, suc